Controlling calcium and phosphate ion release of 3D printed bioactive ceramic scaffolds: An in vitro study
This paper characterizes in an in vitro setting the release of calcium (Ca) and phosphate (PO4) of 3D printed bioactive ceramic scaffold prepared from extrudable paste containing hydroxyapatite and β-tricalcium phosphate (β-TCP). Hydroxyapatite and β-TCP were calcined at 800 °C for 11 h, fabricated into four experimental groups (100% HA, 100% β-TCP, 15%/85% HA/β-TCP, and 15%/85% HA/β-TCP (design)), sintered to 1100 °C for 4 h. Calcium and phosphorus concentrations were evaluated using ICP spectroscopy, and the release of Ca and PO4 ions during dissolution of the CaP-based scaffolds was measured by submerging in 0.05 mol/L Tris(hydroxymethyl)aminomethane-HCl and maintaining a temperature of 37 °C. The Ca and PO4 concentrations of the solutions were measured with the utilization of a calcium assay kit and a phosphate assay kit and read in a UV–visible spectrophotometer. The 100% HA scaffold group showed the greatest concentration of Ca ions (~1.9 mg/dL), but ultimately released at a lower amount as time increased; the 100% HA scaffold also showed the lowest total amount of calcium ions released over the course of evaluation. The results for the 100% β-TCP were on the opposite of the HA with the highest amount of calcium ion release over the study. While the PO4 ion release showed a similar trend as those observed with Ca ions with an apparent difference in the 100% HA scaffold group. There was nearly 0 mg/dL of the phosphate ions released in the first 24 h, in comparison to the amount of Ca ions released during the same time frame. Since various formulations can lead to different properties of these bioactive ceramic scaffolds, it is important to understand how the tailoring of this important biphasic material can impact the long-term outcome of an ever-important in vivo clinical trial in the future.
Keywords3D printing β-TCP scaffolds in vitro calcium phoshpate
- Ducheyne P, Cuckler JM. Bioactive ceramic prosthetic coatings. Clin Orthop Relat R 1992, 76: 102–114.Google Scholar
- Witek L, Smay J, Silva NRFA, et al. Sintering effects on the chemical and physical properties of bioactive ceramic rods biomaterials and biomimetics. New York University, 2011.Google Scholar
- Radin SR, Ducheyne P. Plasma spraying induced changes of calcium phosphate ceramic characteristics and the effect on in vitro stability. J Mater Sci: Mater Med 1992, 3: 33–42.Google Scholar
- De Groot K, Klein C, Wolke JGC, et al. Plasma-sprayed coatings of calcium phosphate. CRC Handbook of Bioactive Ceramics 1990, 2: 133–142.Google Scholar
- Vasiliu CEC. Assembly of hydroxy apatite: β tricalcium phosphate: Calcium sulfate bone engineering scaffolds. Master Thesis. Oklahoma State University, 2008.Google Scholar
- Simon JL, Michna S, Lewis JA, et al. In vivo bone response to 3D periodic hydroxyapatite scaffolds assembled by direct ink writing. J Biomed Mater Res 2007, 83A: 747–758.Google Scholar
- Mijares DQ. Synthetic bone mineral (SBM): Prevention of bone loss induced by estrogen deficiency in a rat model. New York: NYU College of Dentistry, 2009.Google Scholar
- Taylor JC, Hinczak I. Rietveld made easy: A practical guide to the understanding of the method and successful phase quantifications. Sietronics Pty Limited, 2006. Available at http://www.ccp14.ac.uk/ccp/web-mirrors/commercial/siro quant/siroqnt/pdfs/rmeintro.pdf.Google Scholar
- Rietveld HM. The Rietveld Method. Oxford University Press, 1993.Google Scholar
- Nilen RWN, Richter PW. The thermal stability of hydroxyapatite in biphasic calcium phosphate ceramics. J Mater Sci: Mater Med 2008, 19: 1693–1702.Google Scholar
- Sweet L, Kang Y, Czisch C, et al. Geometrical versus random β-TCP scaffolds: Exploring the effects on Sschwann cell growth and behavior. PLoS ONE 2015, 10: e0139820.Google Scholar
Open Access The articles published in this journal are distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.